- Nano Express
- Open Access
Acceptor formation in Mg-doped, indium-rich Ga x In1−xN: evidence for p-type conductivity
© Balkan et al.; licensee Springer. 2012
- Received: 18 July 2012
- Accepted: 12 September 2012
- Published: 18 October 2012
We report on the Mg-doped, indium-rich Ga x In1−xN (x < 30). In the undoped material, the intrinsic electron density is very high and as a result there is no detectable photoconductivity (PC) signal within the range of temperatures of 30 < T < 300 K. In the Mg-doped material however, where the conductivity is reduced, there is a strong PC spectrum with two prominent low-energy peaks at 0.65 and 1.0 eV and one broad high-energy peak at around 1.35 eV. The temperature dependence of the spectral photoconductivity under constant illumination intensity, at T > 150 K, is determined by the longitudinal-optical phonon scattering together with the thermal regeneration of non-equilibrium minority carriers from traps with an average depth of 103 ± 15 meV. This value is close to the Mg binding energy in GaInN. The complementary measurements of transient photoluminescence at liquid He temperatures give the e-A0 binding energy of approximately 100 meV. Furthermore, Hall measurements in the Mg-doped material also indicate an activated behaviour with an acceptor binding energy of 108 ± 20 meV.
During the last decade, there has been intense research activity in indium-rich GaInN. The reason for the interest lies, primarily, in the unusual optoelectronic properties of these semiconductors, where alloying InN with AlN and GaN extends the operational spectrum of the nitride-based optoelectronic devices from the ultraviolet to the near infrared region covering wavelengths from 200 to 1,650 nm [1–3]. Until a few years ago, the commonly accepted value for the InN band gap energy was 1.89 eV , but the majority of the results were obtained on samples grown by sputtering technique and were characterised as having a polycrystalline structure. Moreover, most of the theoretical work reported at the time was based on this wrong value for the band gap. In 2001 Inushima et al. reported a much lower value of EG = 1.1 eV for the molecular beam epitaxy (MBE)-grown samples . Davydov et al.  performed optical absorption and photoluminescence measurements and reported band gap energy of 0.9 eV. Further improvement in the growth techniques has led to the availability of high quality material. Wu et al.  found a value for the band gap between 0.7 and 0.8 eV from their photo-modulated reflectance and photoluminescence (PL) measurements. Since then a large number of papers from different research groups have been published reporting a value between 0.65 and 0.9 eV in the MBE-grown material. It is interesting to note that none of these groups could detect any peak at 1.9 eV. The band gap variation with temperature has been addressed in some publications with no apparent overall agreement on the actual behaviour. Wu et al.  showed a slight increase in energy with increasing temperature, which is in contrast with the behaviour of most direct semiconductors. However, Davydov et al.  reported a more orthodox dependence, with a reduction of 23 meV in energy when the temperature is increased from 77 to 300 K.
Here, m0, m*, and n are the electron mass, GaInN effective mass and carrier concentration respectively. Since the revision of its band gap, the work on InN and indium-rich GaInN has been primarily focused on their optical properties, and only very limited work on their electrical properties has been reported [2, 3].
As-grown InN epilayers show n-type behaviour which is independent of the growth technique. The situation is similar to the case of GaN, and analogous explanations have been tentatively given to account for the background carrier concentration [1–10]. The reduction in the background carrier density and increase in the mobility were achieved recently, and electron densities as low as 4 × 1019 cm−3 were obtained with metalorganic vapour phase epitaxy (MOVPE) . However, the best results in terms of electron density and carrier mobility were achieved using MBE. It has also been shown that the Hall mobility increases with increasing layer thickness in both MBE and MOVPE samples. This is believed to be due to the reduction in the defect density with increasing thickness . Higashiwaki and Matsui  found, however, that the improvement in Hall mobility with increasing thickness is valid up to a critical thickness value of 150 nm, above which the mobility is approximately constant. It was recently shown that irradiation of InN films with 2 MeV He+ ions followed by thermal annealing below 500°C creates films with high electron concentrations and mobilities . Recently, Lu et al.  have reported that the Hall carrier density does not approach zero as the layer thickness decreases. In order to explain their observations, they suggested the existence of more than one conducting layer, one of which was a surface charge layer, to explain the capacitance-voltage measurements . This hypothesis was also confirmed by high-resolution electron energy loss spectroscopy [16–18]. The work shows clearly the surface electron accumulation which is interpreted as the consequence of donor-type surface states pinning the surface Fermi level above the conduction band minimum.
There have been few early attempts to dope indium-rich GaInN and InN p-type using Mg, but they were unsuccessful . The high electron concentration requires a high Mg doping level to achieve compensation. However, increasing Mg concentration results in a higher defect density. This degrades the surface morphology and crystal quality. Furthermore, the presence of an n-type surface conducting channel screens out the effect of doping of the bulk layer with Mg. However, Jones et al. have recently demonstrated p-type doping using capacitance-voltage (C-V) profiling measurements . They also observed a small photoconductivity signal in Mg-doped GaInN in the entire composition range . Further evidence for successful p doping of In-rich GaInN has been reported by various groups recently [22, 23].
The current work presented here is, to our knowledge, the first study of spectral photoconductivity in Mg-doped, indium-rich GaInN and InN. The photoconductivity (PC) results, coupled with the transient PL and Hall measurements, provide direct evidence for the formation of p-type conducting channels in Mg-doped GaInN.
We have studied the Hall effect in undoped and Mg doped samples in darkness and investigated the spectral photoconductivity and photoluminescence in indium-rich GaInN grown by MBE. The temperature dependence of the DC conductivity in Mg-doped GaInN is explained using a multi-channel conduction mechanism, involving p-doped layers in parallel with the n layer. Temperature dependence of photoconductivity is analysed using the trap dynamics of photo-generated carriers in conjunction with optical phonon-assisted momentum relaxation mechanism. Complementary measurements of the transient photoluminescence at low temperatures are carried out to study e-A transitions in Mg-doped GaInN.
Results and discussion
The samples were grown by a Varian GEN-II gas-source MBE system on (0001) sapphire substrates with a few hundred nanometre-thick AlN buffer layer. This was followed by the growth of Ga x In1−xN epilayers at around 470°C with a growth rate of approximately 0. 6 μm/ h. The undoped sample (GS 1509) had 30% Ga and the Mg-doped one (GS1989) had 20% Ga. The other undoped sample which was used in the PL measurements (GS 1508) had a similar composition to the Mg-doped sample.
Hall measurements were carried out in darkness in the temperature range between T = 9 and 300 K. The current flowing through the sample was kept relatively low (I < 50 μA) to ensure ohmic conditions. Both the mobility and carrier concentration were found to be independent of current and magnetic field at all temperatures.
The temperature behaviour of Hall data which is similar to ours is commonly interpreted in the literature in terms of two parallel conducting channels as described by Jones et al.  and Mahboob et al. [16, 17] as an electron accumulation layer on the surface and a 3-D bulk layer. However, variable magnetic field Hall measurements and the quantitative mobility spectrum analysis  of the Hall data must be considered in order to distinguish the contribution of each channel though the analysis which may be further complicated as a result of the small discrepancy between the electron densities and the mobilities in the two channels .
where ne and μe, are the electron density and the mobility in the GaInN accumulation layer, and p and μp are the hole density and mobility in the p-channels of the bulk layer. Here it is assumed that the electron density in the n-type regions in the bulk (nB) is negligible compared to the surface accumulation density (nB<< ne).
At higher temperatures according to Equations 1 and 2, the measured Hall carrier density and mobility will be the complicated functions of temperature as determined by the temperature dependence of the effective scattering mechanisms in the accumulation layer and the bulk. However, the temperature dependence of the Hall density will be primarily due to the thermally activated behaviour of the holes as we have observed in Figure 3. As a result the activation energy obtained from Figure 3 should correspond to the Mg binding energy.
Since the conductivity in the p-type material is about a factor of 100 smaller than the corresponding undoped material, it is possible to have a detectable spectral PC in the Mg-doped material. We carried out the PC spectrum measurements on both the undoped and the Mg-doped samples at temperatures between T = 33 and 300 K. In the measurements a focused beam of light from a halogen lamp was dispersed using a 0.5-m monochromator. A small fraction of the dispersed light from the monochromator was then split and directed onto a pyroelectric detector to monitor the excitation intensity. The rest of the light was directed onto the sample. A dc voltage was applied to the sample with a series resistor, and the PC signal was detected using a lock-in amplifier. Spectral photoconductivity was measured as a function of temperature under constant illumination intensity. Therefore, to the first approximation, we assume that the photo-generated carrier density is independent of temperature. Therefore, the change in the photoconductivity with temperature is attributed to temperature dependence of the photo-generated carrier mobility.
The main features of the PC spectra are the presence of three broad peaks at E approximately 0.65 eV (λ approximately 1.90 μm), E approximately 1.00 eV (λ approximately 1.24 μm) and E approximately 1.40 eV (λ approximately 0.89 μm). The peak at 1.00 eV corresponds to band-to-band transitions with the nominal indium concentration of 80% [31, 34]. This is commonly accepted value for the band gap of approximately 1.0 eV for Ga0.2In0.8 N. The other two peaks may be explained tentatively in terms of a non uniform composition probably associated with indium segregation. The 1.90-μm peak may be due to the Ga-deficient regions with band-to-band transition energy of 0.65 eV corresponding to the InN band gap [34, 35]. The higher energy peak at 1.4 eV may be the regions with reduced average indium concentration of 50% [31, 34]. The broad nature of the PC peaks does not allow the identification or the existence of the Mg-related transitions.
It is clear from Figure 5 that the peak wavelengths of the PC peaks have no notable temperature dependence. This observation is similar to the behaviour of PL spectra as reported in literature, where there is an extremely weak dependence of the PL peak on temperature . The intensities of PC peaks, however, depend strongly on the temperature of the measurements particularly at temperatures T > 90 K where PC drops rapidly with increasing temperature.
where e, μ e and μ h are the electronic charge, electron and hole mobilities respectively.
where q, α, I and hν are the quantum efficiency, absorption coefficient, intensity of the light absorbed and the photon energy respectively.
where τ p is the minority carrier radiative lifetime for holes.
Where Δp0 is the excess hole density in the steady state.
When the illumination intensity is low or the thermal equilibrium hole density (p0) is high, i.e.
Δσ0 < σ and Δp0 < p0
Photoconductivity will increase linearly with intensity. However, the experiments were performed at constant illumination intensity. Therefore, at high temperatures (in the optical phonon scattering regime) when the quantum efficiency, absorption coefficient and the recombination lifetime have weak temperature dependences, the temperature dependence of the PC will be determined primarily by the minority carrier mobility.
Here τ 1 , τ 2 and ΔNS are the average lifetime before the hole is caught in a trap, average lifetime that a hole stays in the trap (de-trapping time) and the excess hole concentration in the trap.
Space charge neutrality requires Δn0 = Δp0 + ΔNs0.
Here ε ∞ = 8.4 ε ∞ and = ε s = 15.3 ε0 are the high frequency and static permittivity, respectively.
Since the optical phonon energy in indium-rich GaInN is ℏω LO = 72 meV[2, 3] the hole traps will have an average depth from the valence band edge of Eth = 103 ± 15 meV. This value is very close to the Mg binding energy in indium-rich GaInN obtained from the C-V and variable magnetic field Hall measurements, in [23, 39] and from Figure 3.
We have investigated dark (DC) and photo (PC) conductivity and PL in indium-rich GaInN grown by MBE. To our knowledge this is the first spectral measurements of photoconductivity in Mg-doped GaInN. Our results indicate that indium segregation may be responsible for the non uniform composition giving rise to three broad peaks in the photoconductivity spectra. From the temperature dependence of the photoconductivity, an average trap energy of Eth = 103 ± 15 meV is obtained. Complementary measurements of the transient PL at low temperatures shows e-A transitions with the acceptor binding energy of approximately 100 meV. The temperature dependence of the DC conductivity in Mg-doped GaInN is explained using a multi-channel conduction mechanism, involving p-doped layers in parallel with the n layer, with an acceptor ionisation energy of 108 ± 20 meV. This is also in excellent agreement with the PC and PL results.
We are grateful to WJ Schaff for the samples, to TUBITAK Ankara for the funding (project number EEEAG-105E076) and to Istanbul University for the funding (project number 9571). We also acknowledge the COST Action MP 0805 for funding the international scientific collaboration.
- Yim JWL, Jones RE, Yu KM, Ager JW, Walukiewicz W, Schaff WJ, Wu J: Effects of surface states on electrical characteristics of InN and In1−xGaxN. Phys Rev B 2007, 76: 041303.View ArticleGoogle Scholar
- Zanato D, Balkan N, Ridley BK, Hill G, Schaff WJ: Hot electron cooling rates via the emission of LO-phonons in InN. Semicond Sci Technol 2004, 19(8):1024–1028. 10.1088/0268-1242/19/8/013View ArticleGoogle Scholar
- Tiras E, Zanato D, Mazzucato S, Balkan N, Schaff WJ: In-plane photovoltage measurements on MBE grown InN. Superlattices Microstruct 2004, 36: 473–485. 10.1016/j.spmi.2004.10.003View ArticleGoogle Scholar
- Tansley TL, Foley CP: Optical band gap of indium nitride. J Appl Phys 1986, 59: 3241. 10.1063/1.336906View ArticleGoogle Scholar
- Inushima T, Mamutin VV, Vekshin VA, Ivanov SV, Sakon T, Motokawa M, Ohoya S: Physical properties of InN with the band gap energy of 1.1 eV. J Cryst Growth 2001, 227–228: 481–485.View ArticleGoogle Scholar
- Davydov VY, Klochikhin AA, Seisyan RP, Emtsev VV, Ivanov SV, Bechstedt F, Furthmüller J, Harima H, Mudryi AV, Aderhold J, Semchinova O, Graul J: Absorption and emission of hexagonal InN. Evidence of narrow fundamental band gap. Phys Status Solidi B 2002, 229: R1-R3. 10.1002/1521-3951(200202)229:3<R1::AID-PSSB99991>3.0.CO;2-OView ArticleGoogle Scholar
- Wu J, Walukiewicz W, Yu KM, Ager JW III, Aller EE, Lu H, Schaff WJ, Saito Y, Nanishi N: Unusual properties of the fundamental band gap of InN. Appl Phys Lett 2002, 80: 3967. 10.1063/1.1482786View ArticleGoogle Scholar
- Davydov VY, Klochikhin AA, Emtsev VV, Kurdyukov DA, Ivanov SV, Vekshin VV, Bechstedt F, Furthmüller J, Aderhold J, Graul J, Mudryi AV, Harima H, Hashimoto A, Yamamoto A, Haller EE: Band gap of hexagonal InN and InGaN alloys. Phys Status Solidi B 2002, 234: 787–795. 10.1002/1521-3951(200212)234:3<787::AID-PSSB787>3.0.CO;2-HView ArticleGoogle Scholar
- Davydov VY, Klochikhin AA, Emtsev VV, Ivanov SV, Vekshin VV, Bechstedt F, Furthmüller J, Harima H, Mudryi AV, Hashimoto A, Yamamoto A, Aderhold J, Graul J, Haller EE: Band gap of InN and In-rich InxGa1−xN alloys (0.36 < x < 1). Phys Status Solidi B 2002, 230: R4-R6. 10.1002/1521-3951(200204)230:2<R4::AID-PSSB99994>3.0.CO;2-ZView ArticleGoogle Scholar
- Jenkins DW, Dow JD: Electronic structures and doping of InN, InxGa1-xN, and InxAl1-xN. Phys Rev B 1989, 39: 3317. 10.1103/PhysRevB.39.3317View ArticleGoogle Scholar
- Sato M: Carrier density of epitaxial InN grown by plasma-assisted metalorganic chemical vapor deposition. Jpn J Appl Phys 1997, 36: L658-L660. 10.1143/JJAP.36.L658View ArticleGoogle Scholar
- Yamaguchi S, Kariya M, Nitta S, Tacheuchi T, Wetzel C, Amano H, Akasaki I: Structural properties of InN on GaN grown by metalorganic vapor-phase epitaxy. J Appl Phys 1999, 85: 7682. 10.1063/1.370571View ArticleGoogle Scholar
- Higashiwaki M, Matsui T: High-quality InN film grown on a low-temperature-grown GaN intermediate layer by plasma-assisted molecular-beam epitaxy. Jpn J Appl Phys 2002, 41: L540-L542. 10.1143/JJAP.41.L540View ArticleGoogle Scholar
- Jones RE, Li SX, Haller EE, van Genuchten HCM, Yu KM, Ager JW III, Liliental-Weber Z, Walukiewicz W, Lu H, Schaff WJ: High electron mobility InN. Appl Phys Lett 2002, 90: 162103.View ArticleGoogle Scholar
- Lu H, Schaff WJ, Eastman LF, Stutz CE: Surface charge accumulation of InN films grown by molecular-beam epitaxy. Appl Phys Lett 2003, 82: 1736. 10.1063/1.1562340View ArticleGoogle Scholar
- Mahboob I, Veal TD, McConville CF, Lu H, Schaff WJ: Intrinsic electron accumulation at clean InN surfaces. Phys Rev Lett 2004, 92: 036804.View ArticleGoogle Scholar
- Mahboob I, Veal TD, Piper LFJ, McConville CF, Lu H, Schaff WJ, Furthmuller J, Bechsted F: Origin of electron accumulation at wurtzite InN surfaces. Phys Rev B Rapid Comm 2004, 69: 201307.View ArticleGoogle Scholar
- Piper LFJ, Veal TD, Mahboob I, McConville CF, Lu H, Schaff WJ: Origin of the n-type conductivity of InN: the role of positively charged dislocations. Appl Phys Lett 2006, 88: 252109. 10.1063/1.2214156View ArticleGoogle Scholar
- Mamutin VV, Vekshin VA, Davydov VY, Ratnikov VV, Kudriavtsev YA, Ber BY, Emtsev VV, Ivanov SV: Mg-doped hexagonal InN/Al2O3 films grown by MBE. Phys Status Solidi A 1999, 176: 373. 10.1002/(SICI)1521-396X(199911)176:1<373::AID-PSSA373>3.0.CO;2-IView ArticleGoogle Scholar
- Jones RE, Yu KM, Li X, Walukiewicz W, Ager JW, Haller E, Lu H, Schaff WJ: Evidence for p-type doping of InN. Phys Rev Lett 2006, 96: 125505.View ArticleGoogle Scholar
- Schaff WJ, Chen XD, Hao D, Matthews K, Richards T, Eastman LF, Lu H, Cho CJH, Cha HY: Electrical properties of InGaN grown by molecular beam epitaxy. Phys Status Solidi B 2008, 245(5):868. 10.1002/pssb.200778710View ArticleGoogle Scholar
- Kudrawiec R, Suski T, Serafinczuk J, Misiewicz J, Muto D, Nanishi Appl Y: Photoreflectance of InN and InN:Mg layers: an evidence of Fermi level shift toward the valence band upon Mg doping in InN. Appl Phys Lett 2008, 93: 131917. 10.1063/1.2995989View ArticleGoogle Scholar
- Brown GF, Ager JW III, Walukiewicz W, Schaff WJ, Wu J: Probing and modulating surface electron accumulation in InN by the electrolyte gated Hall effect. Appl Phys Lett 2008, 93: 262105. 10.1063/1.3062856View ArticleGoogle Scholar
- Look DC, Lu H, Schaff WJ, Jasinski J, Liliental-Weber Z: Donor and acceptor concentrations in degenerate InN. Appl Phys Lett 2002, 80: 258. 10.1063/1.1432742View ArticleGoogle Scholar
- Ridley BK: Energy exchange in 2D electron–electron collisions with dynamic screening. J Phys Condens Matter 2001, 13: 2799–2805. 10.1088/0953-8984/13/12/304View ArticleGoogle Scholar
- Anderson DR, Zakhleniuk NA, Babiker M, Ridley BK, Bennett CR: Polar-optical phonon-limited transport in degenerate GaN-based quantum wells. Phys Rev B 2001, 63: 245313.View ArticleGoogle Scholar
- Lisesivdin SB, Balkan N, Ozbay E: A simple parallel conduction extraction method (SPCEM) for MODFETs and undoped GaN-based HEMTs. Microelectron J 2008, 40: 413–417.View ArticleGoogle Scholar
- Swartz CH, Tompkins RP, Giles NC, Myers TH, Lu H, Schaff WJ, Eastman LF: Investigation of multiple carrier effects in InN epilayers using variable magnetic field Hall measurements. J Cryst Growth 2004, 269: 29–34. 10.1016/j.jcrysgro.2004.05.030View ArticleGoogle Scholar
- Ager JW, Miller N, Jones RE, Yu KM, Wu J, Schaff WJ, Walukiewicz W: Mg-doped InN and InGaN - photoluminescence, capacitance-voltage and thermopower measurements. Phys Status Solidi B 2008, 245: 873–877. 10.1002/pssb.200778731View ArticleGoogle Scholar
- Ridley BK: Negative Differential Resistance and Instabilities in 2-D Semiconductors. Edited by: Balkan N, Ridley BK, Vickers AJ. New York: Plenum; 1993:1–21.View ArticleGoogle Scholar
- Tiras E, Gunes M, Balkan N, Airey R, Schaff WJ: Superconductivity in heavily compensated Mg-doped InN. Appl Phys Lett 2009, 94: 142108. 10.1063/1.3116120View ArticleGoogle Scholar
- King PDC, Veal TD, Jefferson PH, McConville CF, Hai L, Schaff WJ: Variation of band bending at the surface of Mg-doped InGaN: evidence of p-type conductivity across the composition range. Phys Rev B 2007, 75: 115312.View ArticleGoogle Scholar
- Kane MJ, Apsley N, Anderson DA, Taylor LL, Kerr T: Parallel conduction in GaAs/AlxGa1−xAs modulation doped heterojunctions. J Phys C: Solid State Phys 1985, 18: 5629–5636. 10.1088/0022-3719/18/29/013View ArticleGoogle Scholar
- Wu J, Walukiewicz W, Yu KM, Ager JW, Haller EE, Lu H, Schaff WJ: Small band gap bowing in In1−xGaxN alloys. Appl Phys Lett 2002, 80: 4741–4743. 10.1063/1.1489481View ArticleGoogle Scholar
- Veal TD, Jefferson PH, Piper LFJ, McConville CF, Joyce TB, Chalker PR, Considine L, Lu H, Schaff WJ: Transition from electron accumulation to depletion at InGaN surfaces. J Appl Phys Lett 2006, 89: 202110. 10.1063/1.2387976View ArticleGoogle Scholar
- Mazzucato S, Balkan N, Teke A, Erol A, Potter RJ, Arikan MC, Marie X, Fontaine C, Carrere H, Bedel E, Lacoste G: In-plane photovoltaic and photoconductive effects on GaInAs and GaInNAs double quantum well structures. J Appl Phys 2003, 93(5):2440–2448. 10.1063/1.1541104View ArticleGoogle Scholar
- Smith RA: Semiconductors. Cambridge: Cambridge University Press; 1978.Google Scholar
- Kremer RE, Arikan MC, Abele JC, Blakemore JS: Transient photoconductivity measurements in semi‐insulating GaAs. I. An analog approach. J Appl Phys 1987, 62: 2424. 10.1063/1.339849View ArticleGoogle Scholar
- Anderson PA, Swartz CH, Carder D, Reeves RJ, Durbin SM, Chandril S, Mayers TH: Buried p-type layers in Mg-doped InN. Appl Phys Lett 2006, 89: 184104. 10.1063/1.2378489View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.